Please copy and paste this embed script to where you want to embed

N a t t i S. R a o Gunter

D

e

f o r 2nd

s

Schumacher

i

g

n

P l a s t i c s

F

o

r

m

u

l

a

s

E n g i n e e r s

Edition

HANSER Hanser Pubsilhers, Muncih • Hanser Gardner Pubcil ato i ns, Cn i cn i nati

The Authors: Dr.-Ing. Natti S. Rao, 327 Route 216, Ghent, NY 12075, USA Dr. Gunter Schumacher, Am Bollerweg 6, 75045 Walzbachtal-Johlingen, Germany Distributed in the USA and in Canada by Hanser Gardner Publications, Inc. 6915 Valley Avenue, Cincinnati, Ohio 45244-3029, USA Fax: (513) 527-8801 Phone: (513) 527-8977 or 1-800-950-8977 Internet: http://www.hansergardner.com Distributed in all other countries by Carl Hanser Verlag Postfach 86 04 20, 81631 Munchen, Germany Fax: +49 (89) 98 48 09 Internet: http://www.hanser.de The use of general descriptive names, trademarks, etc., in this publication, even if the former are not especially identified, is not to be taken as a sign that such names, as understood by the Trade Marks and Merchandise Marks Act, may accordingly be used freely by anyone. While the advice and information in this book are believed to be true and accurate at the date of going to press, neither the authors nor the editors nor the publisher can accept any legal responsibility for any errors or omissions that may be made. The publisher makes no warranty, express or implied, with respect to the material contained herein. Library of Congress Cataloging-in-Publication Data Rao, Natti S. Design formulas for plastics engineers.-- 2nd ed. / Natti S. Rao, Gunter Schumacher. p. cm. Includes bibliographical references and index. ISBN 1-56990-370-0 (pbk.) 1. Plastics. I. Schumacher, Gunter. II. Title. TPl 140.R36 2004 668.4-dc22 2004017192

Bibliografische Information Der Deutschen Bibliothek Die Deutsche Bibliothek verzeichnet diese Publikation in der DeutschenNationalbibliografie; detaillierte bibliografische Daten sind im Internetiiber abrufbar. ISBN 3-446-22674-5

All rights reserved. No part of this book may be reproduced or transmitted in any form or by any means, electronic or mechanical, including photocopying or by any information storage and retrieval system, without permission in wirting from the publisher.

© Carl Hanser Verlag, Munich 2004 Production Management: Oswald Immel Typeset by Manuela Treindl, Laaber, Germany Coverconcept: Marc Muller-Bremer, Rebranding, Munchen, Germany Coverdesign: MCP • Susanne Kraus GbR, Holzkirchen, Germany Printed and bound by Druckhaus "Thomas Miintzer", Bad Langensalza, Germany

Preface

Today, designing of machines and dies is done to a large extent with the help of computer programs. However, the predictions of theses programs do not always agree with the practical results, so that there is a need to improve the underlying mathematical models. Therefore, knowledge of the formulas, on which the models are based and the limits of their applicability is necessary if one wants to develop a new program or improve one already in use. Often the plastics engineer has to deal with different fields of engineering. The search for the appropriate equations in the various fields concerned can be time-consuming. A collection of formulas from the relevant fields and their applications, as given in this book, make it easier to write one's own program or to make changes in an existing program to obtain a better fit with the experiments. It is often the case that different equations are given in the literature on plastics technology for one and the same target quantity. The practicing engineer is sometimes at a loss judging the validity of the equations he encounters in the literature. During his long years of activity as an R&D engineer in the polymer field at the BASF AG and other companies, Natti Rao tested many formulas published while solving practical problems. This book presents a summary of the important formulas and their applications, which Natti Rao, in cooperation with the well-known resin and machine manufacturers, successfully applied to solve design and processing problems. The formulas are classified according to the fields, rheology, thermodynamics, heat transfer, and part design. Each chapter covers the relevant relations with worked-out examples. A separate chapter is devoted to the practical equations for designing extrusion and injection molding equipment with detailed examples in metric units. In addition, this work contains new, straightforward, practical relationships that have been developed and tested in recent years in solving design problems in the area of extrusion and injection molding. The topic of polymer machine design has been dealt with in several books. However, in these books the know-how was presented in a way that the vast majority of plastics engineers cannot easily apply it to the problems in their day-to-day work. By means of thoroughly worked-out, practical examples this book elucidates the computational background of designing polymer machinery in a manner which every engineer can understand and easily apply in daily practice. We wish to express our thanks to our colleagues at the University of Massachusetts at Lowell, USA, for fruitful discussions. Our thanks are also due to Faculty Innovation Center of the University of Austin, Texas, USA, for help in preparing the manuscript. Austin, USA Karlsruhe, Germany

Natti S. Rao, Ph. D. Gunter Schumacher, Ph. D.

1

Formulas of

Rheology

One of the most important steps in processing polymers is melting the resin, which is initially in the solid state, and forcing the melt through a die of a given shape. During this operation, the melt, whose structure plays a key role in determining the quality of the product to be manufactured, undergoes different flow and deformation processes. The plastics engineer has therefore to deal with the melt rheology, which describes the flow behavior and deformation of the melt. The theory of elasticity and hydromechanics can be considered the frontier field of rheology, because the former describes the behavior of ideal elastic solids, whereas the latter is concerned with the behavior of ideal viscous fluids. Ideal elastic solids deform according to Hooke's Law and ideal viscous fluids obey the laws of Newtonian flow. The latter are also denoted as Newtonian fluids. Plastic melts exhibit both viscous and elastic properties. Thus, the design of machines and dies for polymer processing requires quantitative description of the properties related to polymer melt flow. Starting from the relationships for Hookean solids, formulas describing viscous shear flow of the melt are treated first, as far as they are of practical use in designing polymer machinery. This is followed by a summary of expressions for steady and time-dependent viscoelastic behavior of melts.

1.1

Ideal Solids

The behavior of a polymer subjected to shear or tension can be described by comparing its reaction to external force with that of an ideal elastic solid under load. To characterize ideal solids, first of all it is necessary to define certain quantities as follows [I]: The axial force Fn in Figure 1.1 causes an elongation A/ of the sample of diameter dQ and length I0 that is fixed at one end. Following equations apply for this case: Engineering strain: (Li) Hencky strain: (1.2) Tensile stress: (1.3)

Figure 1.1

Deformation of a Hookean solid by a tensile stress [1 ]

Reference area: (1.4) Poisson's ratio: (1.5) Figure 1.2 shows the influence of a shear force Fv acting on the area A of a rectangular sample causing the displacement AU. The valid expressions are defined by: Shear strain: (1.6) Shear stress: (1.7)

Figure 1.2

Deformation of a Hookean solid by shearing stress [1 ]

P

VtrbV

Figure 1.3

P

Hookean solid under compression [1]

The isotropic compression due to the pressure acting on all sides of the cube shown in Figure 1.3 is given by the engineering compression ratio K (1.8) where AV is the reduction of volume of a body with the original volume V0 due to deformation. 1.1.1

Hooke'sLaw

The linear relationships between stress and strain of a Hookean solid are given by [I]. (1.9) (1.10) (1.11) Where E is the modulus of elasticity, G is the shear modulus, and K is the bulk modulus. These moduli are constant for a Hookean solid. In addition, the relationship existing between £, G and K is expressed as [ 1 ] (1.12) For an incompressible solid this leads (K —», jl —> 0.5) to [1]

E = 3G

1.2

(1.13)

N e w t o n i a n Fluids

There is a linear relationship between stress and strain in the case of Newtonian fluids similar to the one for ideal elastic solids. The fluid between the upper plate in Figure 1.4 is moving at a constant velocity Ux and the lower stationary plate experiences a shear stress T (see also Figure 1.2).

Ux

H

y x Figure 1.4

Shear flow

(1.14) The shear or deformation rate of the fluid is equal to (1.15) The shear viscosity is defined as (1.16) For an extensional flow, which corresponds to the tension test of a Hookean solid, we get (1.17) where 1, only the first term of these equations is significant. Therefore, for the heating or cooling time we obtain [2] Plate:

Cylinder:

Sphere:

(3.38)

(3.39)

(3.40) The solutions of Equation 3.32 to Equation 3.37 are presented in a semi-logarithmic plot in Figure 3.9, in which the temperature ratio 0 ^ = (T w - T b )/(T W - Ta) is shown as a function of the Fourier number F0. Not considering small Fourier numbers, these plots are straight lines approximated by Equation 3.38 to Equation 3.40. If the time tk is based on the centre line temperature Th instead of the average temperature fb, we get [3] (3.41) Analogous to Figure 3.9, the ratio 0 ^ with the centre line temperature Tb at time tk is plotted in Figure 3.10 over the Fourier number for bodies of different geometry [4].

Temperature ratio 6fb

c

b Q

Temperature ratio &jb

Fourier number F0 Figure 3.9 Average temperature of an infinite slab (c), a long cylinder (b) and a sphere (a) during non-steady heating of cooling [2]

Figure 3.10

Fourier number F^otZX1 Axis temperature for multidimensional bodies [4]

The foregoing equations apply to cases, in which the thermal resistance between the body and the surroundings is negligibly small (OC0 -»), for example, in injection molding between the part and the coolant. This means that the Biot number should be very large, Bi —» oo. The Biot number for a plate is (3.42) where a a = heat transfer coefficient of the fluid X = thermal conductivity of the plastic As the heat transfer coefficient has a finite value in practice, the temperature ratio 0 r based on the centre line temperature, is given in Figure 3.11 as a function of the Fourier number with the reciprocal of the Biot number as parameter [5]. Example 1 [6] Cooling of a part in an injection mold for the following conditions: Resin: LDPE Thickness of the plate: s =12.7 mm Temperature of the melt: Ta = 243.3 0 C Mold temperature: T w = 21.1 0 C Demolding temperature: Tb = 76.7 0 C Thermal diffusivity: a =1.29 10~3 cm2/s The cooling time tk is to be calculated. Solution The temperature ratio 0 T b :

Fourier number F 0 from Figure 3.10 at 0 T b = 0.25 P 0 = 0.65 cooling time tk:

Example 2 [6] Calculate the cooling time tk in Example 1 if the mold is cooled by a coolant with a heat transfer coefficient of a a = 2839 W/(m 2 • K). Solution

The resulting Biot number is — = 0.01342 Bi As can be extrapolated from Figure 3.11, the Fourier number does not differ much from the one in the previous example for &Th = 0.25 and 1/Bi = 0.01342. The resistance due to convection is therefore negligible and the cooling time remains almost the same. However, the convection resistance has to be taken into account in the case of a film with a thickness of 127 jU that is cooling in quiescent air, as shown in the following calculation: The heat transfer coefficient for this case is approximately

The Biot number Bi

P 0 from Figure 3.11 F0 = 95

The cooling time

Example 3 [7] Cooling of an extruded wire A polyacetal wire of diameter 3.2 mm is extruded at 190 0 C into a water bath at 20 0 C. Calculate the length of the water bath to cool the wire from 190 0 C to a centre line temperature of 140 0 C. The following conditions are given:

haul-off rate of the wire Vn = 0.5 m/s

Fourier number F0=Q-IZX2 Figure 3.11

Midplane temperature for an infinite plate [5]

Solution The Biot number Bi

where R = radius of the wire B i = 1 7 M - 1 - 6 =11.13 1000 • 0.23

— = 0.0846 Bi

The temperature ratio QTh The Fourier number P 0 for QT = 0.706 and —7 = 0.0846 from Figure 3.11 is approxiBi mately F0 -0.16 The cooling time tk follows from

fk = 4.1s The length of the water bath is

3.2.2

Thermal Contact Temperature

If two semi infinite bodies of different initial temperatures 0 A and QAi are brought into contact as indicated in Figure 3.12, the resulting contact temperature 0 ^ is given by [3]

(3.43)

where = = = =

thermal conductivity density specific heat coefficient of heat penetration

$

1

2 /

Figure 3.12

Temperature distribution in semi infinite solids in contact [3]

Equation 3.43 also applies for the case of contact of short duration between thick bodies. It follows from this equation that the contact temperature depends on the ratio of the coefficients of heat penetration and lies nearer to the initial temperature of body that has a higher coefficient of penetration. The ratio of the temperature differences (0 A - QK) and (0 K - QA ) are inversely proportional to the coefficient of penetration: (3.44)

Example According to Equation 3.43 [8] the contact temperature Qw mold at the time of injection is

of the wall of an injection

(3.45) where

= ^J Ape = temperature before injection = melt temperature Indices w and p refer to mold and polymer, respectively. As shown in Table 3.1 [8], the coefficients of heat penetration of metals are much higher than those of polymer melts. Hence the contact temperature lies in the vicinity of the mold wall temperature before injection. The values given in the Table 3.1 refer to the following units of the properties: thermal conductivity X: W/(m • K) density p: kg/m3 specific heat c: kj/(kg • K)

Table 3.1

Coefficients of Heat Penetration of Mold Material and Resin [8]

Material

Coefficient of heat penetration b Ws 0 5 Hi 2 KT 1

Beryllium copper (BeCu 25) Unalloyed steel (C45W3) Chromium steel (X40Crl3) Polyethylene (HDPE) Polystyrene (PS)

17.2 • 103 13.8 • 103 11.7- 103 0.99 • 103 0.57 • 103

The approximate values for steel are A =50W/(m-K) p =7850kg/m3 c = 0.485 kj/(kg • K) The coefficient of heat penetration b

3.3

H e a t C o n d u c t i o n w i t h Dissipation

The power created by the tangential forces in the control volume of the fluid flow is denoted as dissipation [9]. In shear flow the rate of energy dissipation per unit volume is equal to the product of shear force and shear rate [ 10]. The power due to dissipation [11] therefore is: (3.46) From the power law we get (3.47)

For a Newtonian fluid with n - 1 we obtain (3.48)

The applicable differential equation for a melt flow between two plates, where the upper plate is moving with a velocity Ux (Figure 2.4) and the lower plate is stationary [11] is (3.49)

For drag flow the velocity gradient is given by (3.50) Equation 3.49 can now be written as (3.51) If the temperature of the upper plate is T1 and that of lower plate is T0, the temperature profile of the melt is obtained by integrating Equation 3.51. The resulting expression is (3.52) As shown in Section 4.2.3, this equation can be used to calculate the temperature of the melt film in an extruder.

3.4

Dimensionless G r o u p s

Dimensionless groups can be used to describe complicated processes that are influenced by a large number of variables with the advantage that the entire process can be analyzed on a sound basis by means of a few dimensionless parameters. Their use in correlating experimental data and in scaling-up of equipment is well known. Table 3.2 shows some of the dimensionless groups often used in plastics engineering. Table 3.2

Dimensionless Groups

Symbol

Name

Definition

Bi Br Deb

Biot number Brinkman number Deborah number Fourier number Grashof number Graetz number Lewis number Nahme number Nusselt number Peclet number Prandtl number Reynolds number Sherwood number Schmidt number Stokes number

a Xl Xx 7]w21 (AAT)

F0 Gr Gz Le Na Nu Pe Pr Re Sh Sc Sk

at It g/3-ATflv l2l(a-tv) aid /3T W2T] IX all X wll a vIa pwll T]

PJIS vlS P-II(T]-W)

Nomenclature: a: g: /: p: t.

thermal diffusivity acceleration due to gravity characteristic length ressure time

(m2/s) (m/s2) (m) (N/m ) (s)

Indices D, P: AT: w: O1: /J: /J1: (5S: & Tj: A: v: tv: p:

3.4.1

memory and process of polymer respectively Temperature difference (K) Velocity of flow (m/s) Outside heat transfer coefficient [W/(m 2 • K)] Coefficient of volumetric expansion (K" ) Temperature coefficient in the power law of viscosity (KT1) Mass transfer coefficient (m/s) Diffusion coefficient (m 2 /s) Viscosity (Ns/m 2 ) Thermal conductivity (Index i refers to t h e inside value) [ W / ( m K)] Kinematic viscosity (m 2 /s) Residence time (s) Density (kg/m 3 )

Physical Meaning of Dimensionless Groups

Biot number: Ratio of thermal resistances in series: (/ / A1) / (1 / oQ Application: heating or cooling of solids by heat transfer through conduction and convection Brinkmann number: ratio of heat dissipated (T] w ) to heat conducted (AAT) Application: polymer melt flow Fourier number: ratio of a characteristic body dimension to an approximate temperature wave penetration depth for a given time [16] Application: unsteady state heat conduction Deborah number: ratio of the period of memory of the polymer to the duration of processing [13]. At Deb > 1 the process is determined by the elasticity of the material, whereas at Deb < 1 the viscous behavior of the polymer influences the process remarkably. Grashof number: ratio of the buoyant force g /5 • AT f to factional force (v) Application: heat transfer by free convection Graetz number: ratio of the time to reach thermal equilibrium perpendicular to the flow direction (I2Ia) to the residence time (tv) Application: heat transfer to fluids in motion

Lewis number: ratio of thermal diffusivity (a) to the diffusion coefficient (S) Application: phenomena with simultaneous heat and mass transfer. Nusselt number: ratio of the total heat transferred (a • /) to the heat by conduction (X) Application: convective heat transfer. Pedet number: ratio of heat transfer by convection (pc -w-l) to the heat by conduction

a)

Application: heat transfer by forced convection. Nahme or Griffith number: ratio of viscous dissipation (j3T W2J]) to the heat by conduction (X) perpendicular to the direction of flow Application: heat transfer in melt flow Prandtl number: ratio of the kinematic viscosity (v) to thermal diffusivity (a) Application: convective heat transfer Reynolds number: ratio of the inertial force (p w I) to viscous force (T]) Application: The Reynolds number serves as a criterium to judge the type of flow. In pipe flow, when Re is less than 2300 the flow is laminar. The flow is turbulent at Re greater than about 4000. Between 2100 and 4000 the flow may be laminar or turbulent depending on conditions at the entrance of the tube and on the distance from the entrance [2] Application: fluid flow and heat transfer. Sherwood number: ratio of the resistance to diffusion (/ / S) to the resistance to mass transfer (l/j8 s ) Application: mass transfer problems Schmidt number: ratio of kinematic viscosity (v) to the diffusion coefficient (S) Application: heat and mass transfer problems Stokes number: ratio of pressure forces (p • Z) to viscous forces (rj • w) Application: pressure flow of viscous media like polymer melts. The use of dimensionless numbers in calculating non Newtonian flow problems is illustrated in Section 4.3.3 with an example.

3.5

H e a t Transfer b y C o n v e c t i o n

Heat transfer by convection, particularly by forced convection, plays an important role in many polymer processing operations such as in cooling a blown film or a part in an injection mold, to mention only two examples. A number of expressions can be found in the literature on heat transfer [3] for calculating the heat transfer coefficient a (see Section 3.1.6). The general relationship for forced convection has the form (3.53)

The equation for the turbulent flow in a tube is given by [16] (3.54) where n = 0.4 for heating n = 0.3 for cooling The following equation applies to laminar flow in a tube with a constant wall temperature [3] (3.55) where d{ = inside tube diameter / = tube length The expression for the laminar flow heat transfer to flat plate is [3] (3.56) Equation 3.56 is valid for Pr = 0.6 to 2000 and Re < 105. The equation for turbulent flow heat transfer to flat plate is given as [3] (3.57) Equation 3.57 applies for the conditions: Pr = 0.6 to 2000 and 5 • 105 < Re < 107. The properties of the fluids in the equations above are to be found at a mean fluid temperature. Example A flat film is moving in a coating equipment at a velocity of 130 m/min on rolls that are 200 mm apart. Calculate the heat transfer coefficient a if the surrounding medium is air at a temperature of 50 0 C. Solution The properties of air at 50 0 C are: Kinematic viscosity v = 17.86 • 10"6 m 2 /s Thermal conductivity A = 28.22 • 10"3 W/(m • K) Prandtl number Pr = 0.69

The Reynolds number ReL, based on the length L = 200 mm is

Substituting ReL = 24262 and Pr = 0.69 into Equation 3.56 gives

As the fluid is in motion on both sides of the film, the Nusselt number is calculated according to [3]

For turbulent flow Nu111^ follows from Equation 3.57:

The resulting Nusselt number Nu is

Heat transfer coefficient a results from

3.6

H e a t Transfer b y R a d i a t i o n

Heating by radiation is used in thermoforming processes to heat sheets or films, so that the shaping process can take place. Because at temperatures above 300 0 C a substantial part of the thermal radiation consists of wavelengths in the infrared range, heat transfer by radiation is also termed as infrared radiation [14]. According to the Stefan-Boltzmann law the rate of energy radiated by a black body per unit area es is proportional to the absolute temperature T to the fourth power (Figure 3.13) [I]: (3.58) The Stefan-Boltzmann constant has the value

Figure 3.13 Black body radiation [1]

Figure 3.14 Lambert's law[1]

Figure 3.15 Properties of radiation

Equation 3.58 can also be written as (3.59) where cs = 5.77 W/(m2 • K4) The dependence of the black body radiation on the direction (Figure 3.14) [1] is given by the cosine law of Lambert (3.60) The radiation properties of technical surfaces are defined as (Figure 3.15) [I]: Reflectivity

(3.61)

Absorptivity

(3.62)

Transmissivity

(3.63)

The sum of these fractions must be unity, or p + a+8 =1 The transmissivity 8 of opaque solids is zero so that p + a= 1 The reflectivity of gases p is zero and for those gases which emit and absorb radiation a+8=l Real bodies emit only a fraction of the radiant energy that is emitted by a black body at the same temperature. This ratio is defined as the emissivity e of the body, (3.64)

At thermal equilibrium according to Kirchhoff s identity 8= a

(3.65)

Radiation heat transfer between nonblack surfaces. The net rate of radiant heat exchange between two infinite parallel plates is given by [15] (3.66) where A = area C12 = emissivity factor and is defined by (3.67)

Indices 1 and 2 refer to the two plates. When T2 is much smaller than T1, the heat flow is approximately (3.68) When the heat transfer takes place by radiation and convection, the total heat transfer coefficient can be written as [15] ^total

=

^convection ~*~ ^radiation

where

Example A plastic sheet moving at a speed of 6 m/min is heated by two high-temperature heating elements. Calculate the power required for heating the sheet from 20 0 C to 140 0 C: net enthalpy of the plastic for a temperature difference of 120 0 C: Ah = 70 kj/kg Width of the sheet Thickness Density of the resin Area of the heating element Emissivity of the heater

w s p A £

=600 mm = 250 |i = 900 kg/m 3 = 0.0093 m 2 = 0.9

Solution Heating power Nn: Mass flow rate of the plastic m :

As the area of the heating element is small compared to that of the sheet the equation applies [14]

total area of the heating element Ag = 2 • A so that we have

T = 9.95 100 T = 995 K

3.7

Dielectric H e a t i n g

The dielectric heat loss that occurs in materials of low electrical conductivity when placed in an electric field alternating at high frequency is used in bonding operations, for example, to heat-seal plastic sheets or films. The power dissipated in the polymer is given by [14] (3.69) where Nn= power (W) / = frequency of the alternating field (s"1) C = capacitance of the polymer (farads) E = applied voltage (Volt) 0 = phase angle

The rate of heat generation in a plastic film can be obtained from Equation 3.69 and given as [15] (3.70) where Nn= rate of heat generation (W/m 3 ) £* = dielectric loss factor b = half thickness of the film (\i) Example Given: E / €* b

= 500 V = 10 MHz = 0.24 =50 Ji

Calculate the rate of heat generation and the time required to heat the polymer from 20 0 C to 150 0 C. Substituting the given values in Equation 3.70 gives

The maximum heating rate AT per second is calculated from (3.71) For

Finally the heating time is

3.8

Fick's Law o f Diffusion

Analogous to Fourier's law of heat conduction (Equation 3.1) and the equation for shear stress in shear flow, the diffusion rate in mass transfer is given by Fick's law. This can be written as [16] (3.72) where mA A D^B cA x

= mass flux per unit time - Area = diffusion coefficient of the constituent A in constituent B = mass concentration of component A per unit volume = distance.

The governing expression for the transient rate of diffusion is [2] (3.73) where t = time x = distance The desorption of volatile or gaseous components from a molten polymer in an extruder can be calculated from [17] using Equation 3.73 (3.74) where ^1 Ac C0 D t

= rate of desorption (g/s) = area of desorption (cm2) = initial concentration of the volatile component (g/cm3) in the polymer = diffusion coefficient (cm2/s) - time of exposure (s) of the polymer to the surrounding atmosphere

3.8.1

Permeability

Plastics are permeable by gases, vapors and liquids to a certain extent. The dififiisional characteristics of polymers can be described in terms of a quantity known as permeability.

The mass of the fluid permeating through the polymer at equilibrium conditions is given by [7] (3.75) where m p t A Pv Pi s

- mass of the fluid permeating (g) = permeability [g/(m • s • Pa)] = time of diffusion (s) = area of the film or membrane (m2) = Partial pressures on the side 1 and 2 of the film (Pa) = thickness of the film (mm)

In addition to its dependence on temperature, the permeability is influenced by the difference in partial pressures of the fluid and thickness of the film. Other factors influencing permeability are the structure of the polymer film, such as crystallinity, and the type of fluid. 3.8.2

Absorption and Desorption

The process by which the fluid is absorbed or desorbed by a plastic material is timedependent, governed by its solubility and by the diffusion coefficient [7]. The period until equilibrium value is reached can be very long. Its magnitude can be estimated by the half-life of the process given by [7] (3.76) where t05 = half life of the process s = thickness of the polymer assumed to be penetrated by one side D = diffusion coefficient The value of tQ 5 for moisture in polymethyl methacrylate (PMMA) for and s = 3 mm is 17.1 days when the sheet is wetted from one side only [7]. However, the equilibrium absorption takes much longer, as the absorption rate decreases with saturation.

References [I]

BENDER, E.: Lecture notes, Warme and Stoffiibergang, Univ. Kaiserslautern (1982)

[2]

MCCABE, W. L., SMITH, J. C , HARRIOTT, P.: Unit Operations of Chemical Engineering. McGraw Hill, New York (1985)

[3]

MARTIN, H.: in VDI Warmeatlas, VDI Verlag, Diisseldorf (1984)

[4]

WELTY, J. R., WICKS, C. E., WILSON, R. E.: Fundamentals of Momentum, Heat and Mass Transfer, John Wiley, New York (1983)

[5]

KREITH, E, BLACK, W. Z.: Basic Heat Transfer, Harper & Row, New York (1980)

[6]

THORNE, J. L.: Plastics Process Engineering, Marcel Dekker, New York (1979)

[7]

OGORKIEWICZ, R. M.: Thermoplastics - Properties and Design, John Wiley, New York (1974)

[8]

WUBKEN, G.: Berechnen von Spritzgiefiwerkzeugen, VDI Verlag, Diisseldorf (1974)

[9]

GERSTEN, K.: Einfuhrung in die Stromungsmechanik, Vieweg, Braunschweig (1981)

[ 10] WINTER, H. H.: Extruder als Plastifiziereinheit, VDI Verlag, Diisseldorf (1977) [II] RAUWENDAAL, C.: Polymer Extrusion, Hanser Publishers, Munich (2001) [12] KREMER, H.: Grundlagen der Feuerungstechnik, Engler-Bunte-Institut, Univ. Karlsruhe (1964) [13] COGSWELL, F. N.: Polymer Melt Rheology, George Godwin, London (1981) [ 14] BERNHARDT, E. C.: Processing of Thermoplastic Materials, Reinhold, New York (1959) [15] MCKELVEY, J. M.: Polymer Processing, John Wiley, New York (1962) [16] HOLMAN, J. P.: Heat Transfer, McGraw Hill, New York (1980) [17] SECOR, R. M.: Polym. Eng. ScL 26 (1986) p. 647

4

D e s i g n i n g Plastics

Parts

The deformational behavior of polymeric materials depends mainly on the type and magnitude of loading, time of application of the load, and temperature. The deformation is related to these factors in a complex manner, so that the mathematical treatment of deformation requires a great computational effort [I]. However, in recent times computational procedures for designing plastic parts have been developed using stress-strain data, which were carefully measured by employing computer-aided testing of polymers [2].

4.1

Strength of Polymers

The basic equation for calculating the design stress of a part under load is given by [ 1 ] (4.1) where K av °zui S A

= material strength as a mechanical property = maximum stress occurring in the part ~ allowable stress = factor of safety = material reduction factor

The relation between allowable stress and the polymer-dependent reduction factors can be written as [1] (4.2) The factor A 0 considers the influence of temperature on the strength of the material and can be calculated from [1] (4.3) where 0 = temperature. The limits of applicability of Equation 4.3 are 20 < 0 < 100 0 C. The value k based on the reference temperature of 20 0 C is given for the following materials as[l] PA66 PA6 PBT

=0.0112 = 0.0125 = 0.0095

GR-PA a n d GR-PBT = 0 . 0 0 7 1 POM = 0.0082 ABS =0.0117 The other reduction factors in Equation 4.2 consider the following effects: The factor A st represents the effect of the time of static loading and can have following values depending o n time [ I ] : time

hours

weeks

months

years

Ast

1.3

1.6

1.7

2

The factor A d y n takes the effect of dynamic loading into account and lies in the range of 1.3 to 1.6. The factor A A , considers the influence of aging a n d has to be determined experimentally. The reduction of strength caused by the absorption of moisture by the plastic can be estimated from the factor A w . For unreinforced polyamides A w is roughly [ 1 ] (4.4)

with /ranging from 0 < / < 3 where/= weight percentage of moisture. The value of Aw is 3.4 when/is greater than 3.

4.2

Part Failure

Usually stresses resulting from loading of the part are multiaxial. Because measured material properties do not exist for combined stresses, the multiaxial state has to be reduced to an uniaxial state by applying the principle of equivalence. According to HUBER, VON MISES and HENKY [1] the governing equation for the equivalent stress is (4.5) where CT1, G1 and (T3 are normal stresses. The equivalent strain £ is defined by [3] (4.6) Materials, whose compressive stress is higher than the tensile stress, can be better described by the conical or parabolic criterion [I]. The equivalent stress CT , according to the conical criterion, is given as [ 1 ]

(4.7) The parabolic failure criterion is defined by (4.8)

where m is the ratio of compressive stress to tensile stress. Example Figure 4.1 [1] shows a press fit assembly consisting of a metal shaft and a hub made of POM. The joint strength can be determined as follows: For the numerical values rJrY = 1.6 and p = 22 N/mm 2 the equivalent stress is to be calculated. The tangential stress Gx is given by

Substituing the values above (4.9) The radial compressive stress G1 is

(N]

Figure 4.1 Stress analysis in a press fit hub

Substituting Gx = 50.2 N/mm 2 , G2 = -22 N/mm 2 and G3 = 0 in Equation 4.5 gives

The equivalent stress Cv obtained from

y according

to Equation 4.7 for the conical failure criterion, is

w i t h m = 1.4 for POM. The yield point of POM is around 58 N/mm 2 . Thus, the assumed joint strength is too high. In the case of deformation of the part by shear, the shear stress is given by [I] T = 0.5 O

(4.10)

4.3

T i m e - D e p e n d e n t D e f o r m a t i o n a l Behavior

4.3.1

Short-Term Stress-Strain Behavior

As mentioned in Section 1.4, polymers are viscoelastic materials and their deformational behavior is nonlinear. A typical stress-strain curve of POM under short-term loading is shown in Figure 4.2. Curves of this type can be expressed by a fifth degree polynomial of the form [4] (4.11) where PK0 ... PK5 are polynomial coefficients dependent on the resin at a given temperature.

Stress 6

N/mm2

% Strain £ Figure 4.2

Stress-strain diagram for POM

Stress 6 Figure 4.3

Secant modulus [4]

Strain £

The secant modulus (Figure 4.3) is given by (4.12) Setting PK0 = 0 it follows from Equation 4.11 (4.13) 4.3.2

Long-Term Stress-Strain Behavior

The dimensioning of load bearing plastic components requires knowledge of stress-strain data obtained under long-term loading at different temperatures. Retardation experiments provide data on time-dependent strain in the form of creep plots, see Figure 4.4a. In Figure 4.4b the stress is given as a function of time for different values of strain. Isochronous stress-strain-time curves are illustrated in Figure 4.4c. The critical strain method according to MENGES [10] provides a useful criterion for designing plastic parts. The experiments of MENGES and TAPROGGE [10] show that safe design is possible when the critical strain is taken as the allowable deformation. The corresponding tensile stress can be obtained from the isochronous stress-strain diagram. The expression for calculating the time-dependent strain according to FINDLEY [8] is given as (4.14) The power function of

FINDLEY

[2] is written as (4.15)

The function for the coefficient m is a fifth degree polynomial and that of n is a straight line. With the Findley power function the long-term behavior of plastics up to 105 hours can be described on the basis of measurements covering shorter periods of approx. 103 hours [2].

Strain S

a

Time /

Figure 4.4

Time t Long-term stress-strain behavior [7]

c

Stress 6

Stress 6

b

Strain £

Example [9]

The minimum depth of the simple beam made of SAN shown in Figure 4.5 is to be determined for the following conditions: The beam should support a mid-span load of 11.13 N for 5 years without fracture and without causing a deflection exceeding 2.54 mm.

Figure 4.5

Beam under midspan load [9]

Solution

The maximum stress is given by (4.16)

where P Lybyd

= load (N) = dimensions in (mm) as shown in Figure 4.5

The creep modulus Ec is calculated from (4.17) where /is deflection in mm. The maximum stress from Figure 4.6 after a period of 5 years (= 43800 h) is CJmax 23.44 N/mm 2

Initial applied stress

JL mm2

h Time at rupture Figure 4.6

Creep curve for SAN [9]

Creep modulus

mm2

h Tm iet Figure 4.7

Creep modulus for SAN [9]

Working stress 37 For smaller values of this ratio, Ga1111111118 has to be multiplied by the factor P p given in Figure 5.1. The height H and width W are obtained in this case from Equation 5.6 and Equation 5.7. 5.1.1.2

Shear Rate in Die Channels

The shear rate for the channels treated above can be computed from [3] (5.9)

(5.10)

(5.11) The shear rate for an equilateral triangle is given by [4] (5.12) where d is the half length of a side of the triangle. The relation for a quadratic cross-section is [4] (5.13) where a is the length of a side of the square. In the case of channels with varying cross-sections along the die length, for example, convergent or divergent channels, the channel is divided into a number of sufficiently small increments and the average dimensions of each increment are used in the equations given above [3]. 5.1.1.3

General Relation for Pressure Drop in Any Given Channel Geometry

By means of the substitute radius defined by SCHENKEL [5] the pressure drop in crosssections other than the ones treated in the preceding sections can be calculated. The substitute radius is expressed by [5]

(5.14)

where Rrh= substitute radius A - cross-sectional area B = circumference 5.1.1.4

Examples

The geometrical forms of the dies used in the following examples are illustrated in Figure 5.2. Example 1 It is required to calculate the pressure drop Ap of a LDPE melt at 200 0 C flowing through a round channel, 100 mm long and 25 mm diameter, at a mass flow rate of m = 10 g/s . The constants of viscosity in the Equation 1.36 for the given LDPE are A0 A1 A2 A3 A4

Figure 5.2

= 4.2968 = -3.4709 • 10"1 =-1.1008- 10"1 = 1.4812 • 10"2 =-1.1150-HT 3

Flow channel shapes in extrusion dies

melt density p m = 0.7 g/cm3 Solution Volume flow rate Q = — = — = 14.29 cm 3 /s = 1.429 • 10~5 m 3 /s An 0.7 Shear rate f^ from Equation 5.9:

Shift factor aT from Equation 1.34:

By Equation 1.37, the power law exponent n is

Substituting the constants A1 ... A4 results in n = 1.832 Viscosity 7]a from Equation 1.36

With aT = 0.374, yz = 9.316 and the constants A0 ... A4 we get

Shear stress T from Equation 1.22

Factor of proportionality K from Equation 1.26:

Die constant Gcirde from Equation 5.3:

Pressure drop from Equation 5.2:

Example 2 Melt flow through a slit of width W = 75 mm, height H = 1 mm, and length L = 100 mm. The resin is LDPE with the same viscosity constants as in Example 1. The mass flow rate and the melt temperature have the same values, m = 10 g/s and T = 200 0C. The pressure drop Ap is to be calculated. Solution Volume flow rate Shear rate from Equation 5.10:

Shift factor aT from Equation 1.34: power law exponent n from Equation 1.37: Viscosity 7]a from Equation 1.36: Shear stress T from Equation 1.22: Proportionality factor K from Equation 1.26: Correction factor Fp

As the ratio W/H is greater than 20, the die constant which can be calculated from Equation 5.4 need not be corrected.

and finally the pressure drop Ap from Equation 5.2

Example 3 Melt flow through a slit with width W = 25 mm, height H= 5 mm, and length L = 100 mm. The resin is LDPE with the same viscosity constants as in Example 1. The mass flow rate m = 10 g/s and the melt temperature T = 200 0 C. The pressure drop Ap is to be calculated. Solution Volume flow rate Shear rate ya from Equation 5.10:

Shift factor ar from Equation 1.34:

Power law exponent n from Equation 1.37:

Viscosity 7]a from Equation 1.36:

Shear stress T from Equation 1.22:

Proportionality factor K from Equation 1.26:

Correction factor Fp: As the ratio W/H = 5, which is less than 20, the die constant Gslit has to be corrected. F p from Equation 5.5:

Pressure drop Ap from Equation 5.2:

Example 4 Melt flow through an annulus with an outside radius R0 = 40 mm, an inside radius R1 = 39 mm, and of length L = 100 mm. The resin is LDPE with the same viscosity constants as in Example 1. The process parameters, mass flow rate, and melt temperature remain the same. Solution Volume flow rate Shear rate y^ from Equation 5.11:

Shift factor aT from Equation 1.34:

Power law exponent n from Equation 1.37: n = 2.907 Viscosity 7]a from Equation 1.36: ?7a = 579.43 Pa • s Shear stress T from Equation 1.22: T= 200173.6 N/m 2 Factor of proportionality K from Equation 1.26: K= 1.3410 -10" 13 Correction factor Fp As the ratio G

annuius

from

— = 248.19 is greater than 37, no correction is necessary. Equation 5.8:

Pressure drop Ap from Equation 5.2

Example 5 Melt flow through a quadratic cross section with the length of a side a = 2.62 mm. The channel length L = 50 mm. The resin is LDPE with the following constants for the power law relation in Equation 1.32:

Following conditions are given: mass flow rate melt temperature melt density The pressure drop Ap is to be calculated. Solution Three methods of calculation will be presented to find the pressure drop in this example. Method a With this method, the melt viscosity is calculated according to the power law. Other than that, the method of calculation is the same as in the foregoing examples. Volume flow rate Shear rate For a square with W=H the shear rate yz is

Power law exponent n:

Viscosity rja from Equation 1.32:

Shear stress T from Equation 1.22: T= 40434.88 N/m 2 Proportionality factor K from Equation 1.26: K= 4.568 -1(T14 Correction factor F p W As — = 1 is less than 20, the correction factor is obtained from Equation 5.5 H fp = 1.008 - 0.7474 • 1 + 0.1638 • I 2 = 0.4244 Die constant Gslit from Equation 5.4: Gslit =4.22 • 10"5 G8Ut corrected = 0-4244 • 4.22-10"5 = 1.791 • 10-5 Pressure drop Ap from Equation 5.2:

Method b The shear rate ya is calculated from Equation 5.13

Viscosity ?]a from Equation 1.32: 77a = 24205.54 • 5.67403286"1 = 7546.64 Pa • s Shear stress T from Equation 1.22: T= 42819.6 N/m 2 Power law exponent n from Equation 1.28:

Proportionality factor K from Equation 1.26: K= 4.568 -10" 14 The pressure drop Ap is found from

(5.15)

with the die constant Gsquare

(5.16)

In Equation 5.15

Finally Apsquare from Equation 5.2:

The above relationship for shear rate developed by same result as obtained by Method a.

RAMSTEINER

[4] leads to almost the

Method c In this method, a substitute radius is calculated from Equation 5.14; the pressure drop is then calculated using the same procedure as in the case of a round channel (Example 1): Substitute radius .Rrh:

Shear rate % from Equation 5.13:

Viscosity ?]a from Equation 1.32: 7]a = 24205.54 • 7.1830'3216"1 = 6441.56 Pa • s Shear stress T from Equation 1.22: T = 46269.73 N/m 2 Factor of proportionality from Equation 1.26: K = 4.568- 10"14 ^circle fr°m Equation 5.3:

Pressure drop from Equation 5.2:

This result shows that the relationship, Equation 5.14 [5], is sufficiently accurate for practical purposes. This equation is particularly useful for dimensioning channels, whose geometry differs from the common shape, that is, circle, slit or annulus. The procedure of calculation for an equilateral triangle is shown in the following example: Example 6 Melt flow through an equilateral triangular channel of length L = 50 mm. The side of the triangle 2 d = 4.06 mm. Other conditions remain the same as in Example 5. Solution Substitute radius Rrh from Equation 5.14 with

n = 3.043 RTh= 1.274 mm Shear rate / a from Equation 5.9:

Viscosity 7]a from Equation 1.32: 77a = 24205.54 • 8.8 0 ' 3 2 8 " = 5620.68 Pa • s Shear stress T from Equation 1.22: T= 49462 N/m 2 Factor of proportionality from Equation 1.26: K= 4.568-10"14 Gcircle from Equation 5.3:

Pressure drop Ap from Equation 5.2:

Using the relation developed by RAMSTEINER [4] on the basis of rheological measurement on triangular channels, Example 6 is calculated as follows for the purpose of comparing both methods: Shear rate from Equation 5.12:

Viscosity 7]a from Equation 1.32: 7]a = 24205.54 • 5.6920'3286"1 = 7530.61 Pa • s Shear stress T from Equation 1.22: T = 42864.2 N/m 2 Factor of proportionality from Equation 1.26: K= 4.568 -10" 14

Die constant Gtriangle: (5.17)

Pressure drop Ap from Equation 5.2:

This result differs little from the one obtained by using the concept of substitute radius. Therefore this concept of SCHENKEL [5] is suitable for use in practice. 5.1.1.5

Temperature Rise and Residence Time

The adiabatic temperature increase of the melt can be calculated from (5.18) where AT Ap pm cpm

= = = =

temperature rise (K) pressure difference (bar) melt density (g/cm 3 ) specific heat of the melt kj/(kg • K)

The residence time T of the melt in the die of length L can be expressed as (5.19) u = average velocity of the melt Equation 5.19 for a tube can be written as

(5.20) R = tube radius ya = shear rate according to Equation 5.9

The relation of a slit is (5.21) H = height of slit ya = shear rate according to Equation 5.10 5.1.1.6

Adapting Die Design to Avoid Melt Fracture

Melt fracture can be defined as an instability of the melt flow leading to surface or volume distortions of the extrudate. Surface distortions [34] are usually created from instabilities near the die exit, while volume distortions [34] originate from the vortex formation at the die entrance. Melt fracture caused by these phenomena limits the production of articles manufactured by extrusion processes. The use of processing additives to increase the output has been dealt with in a number of publications given in [35]. However, processing aids are not desirable in applications such as pelletizing and blow molding. Therefore, the effect of die geometry on the onset of melt fracture was examined. The onset of melt fracture with increasing die pressure is shown for LDPE and HDPE in Figure 5.3 [38]. As can be seen, the distortions appear differently depending on the resin. The volume flow rate is plotted in Figure 5.4 [39] first as a function of wall shear stress and then as a function of pressure drop in the capillary for LDPE and HDPE. The sudden increase in slope is evident for LDPE only when the flow rate is plotted against pressure, whereas in the case of HDPE it is the opposite. In addition, for HDPE the occurrence of melt fracture depends on the ratio of length L to diameter D of the capillary. The effect of temperature on the onset of melt fracture is shown in Figure 5.5 [36]. With increasing temperature the onset of instability shifts to higher shear rates. This behavior is used in practice to increase the output. However, exceeding the optimum processing temperature can lead to a decrease in the quality of the product in many processing operations. From these considerations it can be seen that designing a die by taking the resin behavior into account is the easiest method to obtain quality products at high throughputs. Design procedure Using the formulas given in this book and in reference [33], the following design procedure has been developed to suit the die dimensions to the melt flow properties of the resin to be processed with the die. STEP 1: Calculation of the shear rate in the die channel STEP 2: Expressing the measured viscosity plots by a rheological model STEP 3: Calculation of the power law exponent STEP 4: Calculation of the shear viscosity at the shear rate in Step 1 STEP 5: Calculation of the wall shear stress STEP 6: Calculation of the factor of proportionality STEP 7: Calculation of die constant

N/mm2

LDPE

HDPE

Figure 5.3

lrregularties of the extrudate observed at increasing extrusion pressure with LDPE and HDPE [38] InQ

InQ

In

View more...
D

e

f o r 2nd

s

Schumacher

i

g

n

P l a s t i c s

F

o

r

m

u

l

a

s

E n g i n e e r s

Edition

HANSER Hanser Pubsilhers, Muncih • Hanser Gardner Pubcil ato i ns, Cn i cn i nati

The Authors: Dr.-Ing. Natti S. Rao, 327 Route 216, Ghent, NY 12075, USA Dr. Gunter Schumacher, Am Bollerweg 6, 75045 Walzbachtal-Johlingen, Germany Distributed in the USA and in Canada by Hanser Gardner Publications, Inc. 6915 Valley Avenue, Cincinnati, Ohio 45244-3029, USA Fax: (513) 527-8801 Phone: (513) 527-8977 or 1-800-950-8977 Internet: http://www.hansergardner.com Distributed in all other countries by Carl Hanser Verlag Postfach 86 04 20, 81631 Munchen, Germany Fax: +49 (89) 98 48 09 Internet: http://www.hanser.de The use of general descriptive names, trademarks, etc., in this publication, even if the former are not especially identified, is not to be taken as a sign that such names, as understood by the Trade Marks and Merchandise Marks Act, may accordingly be used freely by anyone. While the advice and information in this book are believed to be true and accurate at the date of going to press, neither the authors nor the editors nor the publisher can accept any legal responsibility for any errors or omissions that may be made. The publisher makes no warranty, express or implied, with respect to the material contained herein. Library of Congress Cataloging-in-Publication Data Rao, Natti S. Design formulas for plastics engineers.-- 2nd ed. / Natti S. Rao, Gunter Schumacher. p. cm. Includes bibliographical references and index. ISBN 1-56990-370-0 (pbk.) 1. Plastics. I. Schumacher, Gunter. II. Title. TPl 140.R36 2004 668.4-dc22 2004017192

Bibliografische Information Der Deutschen Bibliothek Die Deutsche Bibliothek verzeichnet diese Publikation in der DeutschenNationalbibliografie; detaillierte bibliografische Daten sind im Internetiiber abrufbar. ISBN 3-446-22674-5

All rights reserved. No part of this book may be reproduced or transmitted in any form or by any means, electronic or mechanical, including photocopying or by any information storage and retrieval system, without permission in wirting from the publisher.

© Carl Hanser Verlag, Munich 2004 Production Management: Oswald Immel Typeset by Manuela Treindl, Laaber, Germany Coverconcept: Marc Muller-Bremer, Rebranding, Munchen, Germany Coverdesign: MCP • Susanne Kraus GbR, Holzkirchen, Germany Printed and bound by Druckhaus "Thomas Miintzer", Bad Langensalza, Germany

Preface

Today, designing of machines and dies is done to a large extent with the help of computer programs. However, the predictions of theses programs do not always agree with the practical results, so that there is a need to improve the underlying mathematical models. Therefore, knowledge of the formulas, on which the models are based and the limits of their applicability is necessary if one wants to develop a new program or improve one already in use. Often the plastics engineer has to deal with different fields of engineering. The search for the appropriate equations in the various fields concerned can be time-consuming. A collection of formulas from the relevant fields and their applications, as given in this book, make it easier to write one's own program or to make changes in an existing program to obtain a better fit with the experiments. It is often the case that different equations are given in the literature on plastics technology for one and the same target quantity. The practicing engineer is sometimes at a loss judging the validity of the equations he encounters in the literature. During his long years of activity as an R&D engineer in the polymer field at the BASF AG and other companies, Natti Rao tested many formulas published while solving practical problems. This book presents a summary of the important formulas and their applications, which Natti Rao, in cooperation with the well-known resin and machine manufacturers, successfully applied to solve design and processing problems. The formulas are classified according to the fields, rheology, thermodynamics, heat transfer, and part design. Each chapter covers the relevant relations with worked-out examples. A separate chapter is devoted to the practical equations for designing extrusion and injection molding equipment with detailed examples in metric units. In addition, this work contains new, straightforward, practical relationships that have been developed and tested in recent years in solving design problems in the area of extrusion and injection molding. The topic of polymer machine design has been dealt with in several books. However, in these books the know-how was presented in a way that the vast majority of plastics engineers cannot easily apply it to the problems in their day-to-day work. By means of thoroughly worked-out, practical examples this book elucidates the computational background of designing polymer machinery in a manner which every engineer can understand and easily apply in daily practice. We wish to express our thanks to our colleagues at the University of Massachusetts at Lowell, USA, for fruitful discussions. Our thanks are also due to Faculty Innovation Center of the University of Austin, Texas, USA, for help in preparing the manuscript. Austin, USA Karlsruhe, Germany

Natti S. Rao, Ph. D. Gunter Schumacher, Ph. D.

1

Formulas of

Rheology

One of the most important steps in processing polymers is melting the resin, which is initially in the solid state, and forcing the melt through a die of a given shape. During this operation, the melt, whose structure plays a key role in determining the quality of the product to be manufactured, undergoes different flow and deformation processes. The plastics engineer has therefore to deal with the melt rheology, which describes the flow behavior and deformation of the melt. The theory of elasticity and hydromechanics can be considered the frontier field of rheology, because the former describes the behavior of ideal elastic solids, whereas the latter is concerned with the behavior of ideal viscous fluids. Ideal elastic solids deform according to Hooke's Law and ideal viscous fluids obey the laws of Newtonian flow. The latter are also denoted as Newtonian fluids. Plastic melts exhibit both viscous and elastic properties. Thus, the design of machines and dies for polymer processing requires quantitative description of the properties related to polymer melt flow. Starting from the relationships for Hookean solids, formulas describing viscous shear flow of the melt are treated first, as far as they are of practical use in designing polymer machinery. This is followed by a summary of expressions for steady and time-dependent viscoelastic behavior of melts.

1.1

Ideal Solids

The behavior of a polymer subjected to shear or tension can be described by comparing its reaction to external force with that of an ideal elastic solid under load. To characterize ideal solids, first of all it is necessary to define certain quantities as follows [I]: The axial force Fn in Figure 1.1 causes an elongation A/ of the sample of diameter dQ and length I0 that is fixed at one end. Following equations apply for this case: Engineering strain: (Li) Hencky strain: (1.2) Tensile stress: (1.3)

Figure 1.1

Deformation of a Hookean solid by a tensile stress [1 ]

Reference area: (1.4) Poisson's ratio: (1.5) Figure 1.2 shows the influence of a shear force Fv acting on the area A of a rectangular sample causing the displacement AU. The valid expressions are defined by: Shear strain: (1.6) Shear stress: (1.7)

Figure 1.2

Deformation of a Hookean solid by shearing stress [1 ]

P

VtrbV

Figure 1.3

P

Hookean solid under compression [1]

The isotropic compression due to the pressure acting on all sides of the cube shown in Figure 1.3 is given by the engineering compression ratio K (1.8) where AV is the reduction of volume of a body with the original volume V0 due to deformation. 1.1.1

Hooke'sLaw

The linear relationships between stress and strain of a Hookean solid are given by [I]. (1.9) (1.10) (1.11) Where E is the modulus of elasticity, G is the shear modulus, and K is the bulk modulus. These moduli are constant for a Hookean solid. In addition, the relationship existing between £, G and K is expressed as [ 1 ] (1.12) For an incompressible solid this leads (K —», jl —> 0.5) to [1]

E = 3G

1.2

(1.13)

N e w t o n i a n Fluids

There is a linear relationship between stress and strain in the case of Newtonian fluids similar to the one for ideal elastic solids. The fluid between the upper plate in Figure 1.4 is moving at a constant velocity Ux and the lower stationary plate experiences a shear stress T (see also Figure 1.2).

Ux

H

y x Figure 1.4

Shear flow

(1.14) The shear or deformation rate of the fluid is equal to (1.15) The shear viscosity is defined as (1.16) For an extensional flow, which corresponds to the tension test of a Hookean solid, we get (1.17) where 1, only the first term of these equations is significant. Therefore, for the heating or cooling time we obtain [2] Plate:

Cylinder:

Sphere:

(3.38)

(3.39)

(3.40) The solutions of Equation 3.32 to Equation 3.37 are presented in a semi-logarithmic plot in Figure 3.9, in which the temperature ratio 0 ^ = (T w - T b )/(T W - Ta) is shown as a function of the Fourier number F0. Not considering small Fourier numbers, these plots are straight lines approximated by Equation 3.38 to Equation 3.40. If the time tk is based on the centre line temperature Th instead of the average temperature fb, we get [3] (3.41) Analogous to Figure 3.9, the ratio 0 ^ with the centre line temperature Tb at time tk is plotted in Figure 3.10 over the Fourier number for bodies of different geometry [4].

Temperature ratio 6fb

c

b Q

Temperature ratio &jb

Fourier number F0 Figure 3.9 Average temperature of an infinite slab (c), a long cylinder (b) and a sphere (a) during non-steady heating of cooling [2]

Figure 3.10

Fourier number F^otZX1 Axis temperature for multidimensional bodies [4]

The foregoing equations apply to cases, in which the thermal resistance between the body and the surroundings is negligibly small (OC0 -»), for example, in injection molding between the part and the coolant. This means that the Biot number should be very large, Bi —» oo. The Biot number for a plate is (3.42) where a a = heat transfer coefficient of the fluid X = thermal conductivity of the plastic As the heat transfer coefficient has a finite value in practice, the temperature ratio 0 r based on the centre line temperature, is given in Figure 3.11 as a function of the Fourier number with the reciprocal of the Biot number as parameter [5]. Example 1 [6] Cooling of a part in an injection mold for the following conditions: Resin: LDPE Thickness of the plate: s =12.7 mm Temperature of the melt: Ta = 243.3 0 C Mold temperature: T w = 21.1 0 C Demolding temperature: Tb = 76.7 0 C Thermal diffusivity: a =1.29 10~3 cm2/s The cooling time tk is to be calculated. Solution The temperature ratio 0 T b :

Fourier number F 0 from Figure 3.10 at 0 T b = 0.25 P 0 = 0.65 cooling time tk:

Example 2 [6] Calculate the cooling time tk in Example 1 if the mold is cooled by a coolant with a heat transfer coefficient of a a = 2839 W/(m 2 • K). Solution

The resulting Biot number is — = 0.01342 Bi As can be extrapolated from Figure 3.11, the Fourier number does not differ much from the one in the previous example for &Th = 0.25 and 1/Bi = 0.01342. The resistance due to convection is therefore negligible and the cooling time remains almost the same. However, the convection resistance has to be taken into account in the case of a film with a thickness of 127 jU that is cooling in quiescent air, as shown in the following calculation: The heat transfer coefficient for this case is approximately

The Biot number Bi

P 0 from Figure 3.11 F0 = 95

The cooling time

Example 3 [7] Cooling of an extruded wire A polyacetal wire of diameter 3.2 mm is extruded at 190 0 C into a water bath at 20 0 C. Calculate the length of the water bath to cool the wire from 190 0 C to a centre line temperature of 140 0 C. The following conditions are given:

haul-off rate of the wire Vn = 0.5 m/s

Fourier number F0=Q-IZX2 Figure 3.11

Midplane temperature for an infinite plate [5]

Solution The Biot number Bi

where R = radius of the wire B i = 1 7 M - 1 - 6 =11.13 1000 • 0.23

— = 0.0846 Bi

The temperature ratio QTh The Fourier number P 0 for QT = 0.706 and —7 = 0.0846 from Figure 3.11 is approxiBi mately F0 -0.16 The cooling time tk follows from

fk = 4.1s The length of the water bath is

3.2.2

Thermal Contact Temperature

If two semi infinite bodies of different initial temperatures 0 A and QAi are brought into contact as indicated in Figure 3.12, the resulting contact temperature 0 ^ is given by [3]

(3.43)

where = = = =

thermal conductivity density specific heat coefficient of heat penetration

$

1

2 /

Figure 3.12

Temperature distribution in semi infinite solids in contact [3]

Equation 3.43 also applies for the case of contact of short duration between thick bodies. It follows from this equation that the contact temperature depends on the ratio of the coefficients of heat penetration and lies nearer to the initial temperature of body that has a higher coefficient of penetration. The ratio of the temperature differences (0 A - QK) and (0 K - QA ) are inversely proportional to the coefficient of penetration: (3.44)

Example According to Equation 3.43 [8] the contact temperature Qw mold at the time of injection is

of the wall of an injection

(3.45) where

= ^J Ape = temperature before injection = melt temperature Indices w and p refer to mold and polymer, respectively. As shown in Table 3.1 [8], the coefficients of heat penetration of metals are much higher than those of polymer melts. Hence the contact temperature lies in the vicinity of the mold wall temperature before injection. The values given in the Table 3.1 refer to the following units of the properties: thermal conductivity X: W/(m • K) density p: kg/m3 specific heat c: kj/(kg • K)

Table 3.1

Coefficients of Heat Penetration of Mold Material and Resin [8]

Material

Coefficient of heat penetration b Ws 0 5 Hi 2 KT 1

Beryllium copper (BeCu 25) Unalloyed steel (C45W3) Chromium steel (X40Crl3) Polyethylene (HDPE) Polystyrene (PS)

17.2 • 103 13.8 • 103 11.7- 103 0.99 • 103 0.57 • 103

The approximate values for steel are A =50W/(m-K) p =7850kg/m3 c = 0.485 kj/(kg • K) The coefficient of heat penetration b

3.3

H e a t C o n d u c t i o n w i t h Dissipation

The power created by the tangential forces in the control volume of the fluid flow is denoted as dissipation [9]. In shear flow the rate of energy dissipation per unit volume is equal to the product of shear force and shear rate [ 10]. The power due to dissipation [11] therefore is: (3.46) From the power law we get (3.47)

For a Newtonian fluid with n - 1 we obtain (3.48)

The applicable differential equation for a melt flow between two plates, where the upper plate is moving with a velocity Ux (Figure 2.4) and the lower plate is stationary [11] is (3.49)

For drag flow the velocity gradient is given by (3.50) Equation 3.49 can now be written as (3.51) If the temperature of the upper plate is T1 and that of lower plate is T0, the temperature profile of the melt is obtained by integrating Equation 3.51. The resulting expression is (3.52) As shown in Section 4.2.3, this equation can be used to calculate the temperature of the melt film in an extruder.

3.4

Dimensionless G r o u p s

Dimensionless groups can be used to describe complicated processes that are influenced by a large number of variables with the advantage that the entire process can be analyzed on a sound basis by means of a few dimensionless parameters. Their use in correlating experimental data and in scaling-up of equipment is well known. Table 3.2 shows some of the dimensionless groups often used in plastics engineering. Table 3.2

Dimensionless Groups

Symbol

Name

Definition

Bi Br Deb

Biot number Brinkman number Deborah number Fourier number Grashof number Graetz number Lewis number Nahme number Nusselt number Peclet number Prandtl number Reynolds number Sherwood number Schmidt number Stokes number

a Xl Xx 7]w21 (AAT)

F0 Gr Gz Le Na Nu Pe Pr Re Sh Sc Sk

at It g/3-ATflv l2l(a-tv) aid /3T W2T] IX all X wll a vIa pwll T]

PJIS vlS P-II(T]-W)

Nomenclature: a: g: /: p: t.

thermal diffusivity acceleration due to gravity characteristic length ressure time

(m2/s) (m/s2) (m) (N/m ) (s)

Indices D, P: AT: w: O1: /J: /J1: (5S: & Tj: A: v: tv: p:

3.4.1

memory and process of polymer respectively Temperature difference (K) Velocity of flow (m/s) Outside heat transfer coefficient [W/(m 2 • K)] Coefficient of volumetric expansion (K" ) Temperature coefficient in the power law of viscosity (KT1) Mass transfer coefficient (m/s) Diffusion coefficient (m 2 /s) Viscosity (Ns/m 2 ) Thermal conductivity (Index i refers to t h e inside value) [ W / ( m K)] Kinematic viscosity (m 2 /s) Residence time (s) Density (kg/m 3 )

Physical Meaning of Dimensionless Groups

Biot number: Ratio of thermal resistances in series: (/ / A1) / (1 / oQ Application: heating or cooling of solids by heat transfer through conduction and convection Brinkmann number: ratio of heat dissipated (T] w ) to heat conducted (AAT) Application: polymer melt flow Fourier number: ratio of a characteristic body dimension to an approximate temperature wave penetration depth for a given time [16] Application: unsteady state heat conduction Deborah number: ratio of the period of memory of the polymer to the duration of processing [13]. At Deb > 1 the process is determined by the elasticity of the material, whereas at Deb < 1 the viscous behavior of the polymer influences the process remarkably. Grashof number: ratio of the buoyant force g /5 • AT f to factional force (v) Application: heat transfer by free convection Graetz number: ratio of the time to reach thermal equilibrium perpendicular to the flow direction (I2Ia) to the residence time (tv) Application: heat transfer to fluids in motion

Lewis number: ratio of thermal diffusivity (a) to the diffusion coefficient (S) Application: phenomena with simultaneous heat and mass transfer. Nusselt number: ratio of the total heat transferred (a • /) to the heat by conduction (X) Application: convective heat transfer. Pedet number: ratio of heat transfer by convection (pc -w-l) to the heat by conduction

a)

Application: heat transfer by forced convection. Nahme or Griffith number: ratio of viscous dissipation (j3T W2J]) to the heat by conduction (X) perpendicular to the direction of flow Application: heat transfer in melt flow Prandtl number: ratio of the kinematic viscosity (v) to thermal diffusivity (a) Application: convective heat transfer Reynolds number: ratio of the inertial force (p w I) to viscous force (T]) Application: The Reynolds number serves as a criterium to judge the type of flow. In pipe flow, when Re is less than 2300 the flow is laminar. The flow is turbulent at Re greater than about 4000. Between 2100 and 4000 the flow may be laminar or turbulent depending on conditions at the entrance of the tube and on the distance from the entrance [2] Application: fluid flow and heat transfer. Sherwood number: ratio of the resistance to diffusion (/ / S) to the resistance to mass transfer (l/j8 s ) Application: mass transfer problems Schmidt number: ratio of kinematic viscosity (v) to the diffusion coefficient (S) Application: heat and mass transfer problems Stokes number: ratio of pressure forces (p • Z) to viscous forces (rj • w) Application: pressure flow of viscous media like polymer melts. The use of dimensionless numbers in calculating non Newtonian flow problems is illustrated in Section 4.3.3 with an example.

3.5

H e a t Transfer b y C o n v e c t i o n

Heat transfer by convection, particularly by forced convection, plays an important role in many polymer processing operations such as in cooling a blown film or a part in an injection mold, to mention only two examples. A number of expressions can be found in the literature on heat transfer [3] for calculating the heat transfer coefficient a (see Section 3.1.6). The general relationship for forced convection has the form (3.53)

The equation for the turbulent flow in a tube is given by [16] (3.54) where n = 0.4 for heating n = 0.3 for cooling The following equation applies to laminar flow in a tube with a constant wall temperature [3] (3.55) where d{ = inside tube diameter / = tube length The expression for the laminar flow heat transfer to flat plate is [3] (3.56) Equation 3.56 is valid for Pr = 0.6 to 2000 and Re < 105. The equation for turbulent flow heat transfer to flat plate is given as [3] (3.57) Equation 3.57 applies for the conditions: Pr = 0.6 to 2000 and 5 • 105 < Re < 107. The properties of the fluids in the equations above are to be found at a mean fluid temperature. Example A flat film is moving in a coating equipment at a velocity of 130 m/min on rolls that are 200 mm apart. Calculate the heat transfer coefficient a if the surrounding medium is air at a temperature of 50 0 C. Solution The properties of air at 50 0 C are: Kinematic viscosity v = 17.86 • 10"6 m 2 /s Thermal conductivity A = 28.22 • 10"3 W/(m • K) Prandtl number Pr = 0.69

The Reynolds number ReL, based on the length L = 200 mm is

Substituting ReL = 24262 and Pr = 0.69 into Equation 3.56 gives

As the fluid is in motion on both sides of the film, the Nusselt number is calculated according to [3]

For turbulent flow Nu111^ follows from Equation 3.57:

The resulting Nusselt number Nu is

Heat transfer coefficient a results from

3.6

H e a t Transfer b y R a d i a t i o n

Heating by radiation is used in thermoforming processes to heat sheets or films, so that the shaping process can take place. Because at temperatures above 300 0 C a substantial part of the thermal radiation consists of wavelengths in the infrared range, heat transfer by radiation is also termed as infrared radiation [14]. According to the Stefan-Boltzmann law the rate of energy radiated by a black body per unit area es is proportional to the absolute temperature T to the fourth power (Figure 3.13) [I]: (3.58) The Stefan-Boltzmann constant has the value

Figure 3.13 Black body radiation [1]

Figure 3.14 Lambert's law[1]

Figure 3.15 Properties of radiation

Equation 3.58 can also be written as (3.59) where cs = 5.77 W/(m2 • K4) The dependence of the black body radiation on the direction (Figure 3.14) [1] is given by the cosine law of Lambert (3.60) The radiation properties of technical surfaces are defined as (Figure 3.15) [I]: Reflectivity

(3.61)

Absorptivity

(3.62)

Transmissivity

(3.63)

The sum of these fractions must be unity, or p + a+8 =1 The transmissivity 8 of opaque solids is zero so that p + a= 1 The reflectivity of gases p is zero and for those gases which emit and absorb radiation a+8=l Real bodies emit only a fraction of the radiant energy that is emitted by a black body at the same temperature. This ratio is defined as the emissivity e of the body, (3.64)

At thermal equilibrium according to Kirchhoff s identity 8= a

(3.65)

Radiation heat transfer between nonblack surfaces. The net rate of radiant heat exchange between two infinite parallel plates is given by [15] (3.66) where A = area C12 = emissivity factor and is defined by (3.67)

Indices 1 and 2 refer to the two plates. When T2 is much smaller than T1, the heat flow is approximately (3.68) When the heat transfer takes place by radiation and convection, the total heat transfer coefficient can be written as [15] ^total

=

^convection ~*~ ^radiation

where

Example A plastic sheet moving at a speed of 6 m/min is heated by two high-temperature heating elements. Calculate the power required for heating the sheet from 20 0 C to 140 0 C: net enthalpy of the plastic for a temperature difference of 120 0 C: Ah = 70 kj/kg Width of the sheet Thickness Density of the resin Area of the heating element Emissivity of the heater

w s p A £

=600 mm = 250 |i = 900 kg/m 3 = 0.0093 m 2 = 0.9

Solution Heating power Nn: Mass flow rate of the plastic m :

As the area of the heating element is small compared to that of the sheet the equation applies [14]

total area of the heating element Ag = 2 • A so that we have

T = 9.95 100 T = 995 K

3.7

Dielectric H e a t i n g

The dielectric heat loss that occurs in materials of low electrical conductivity when placed in an electric field alternating at high frequency is used in bonding operations, for example, to heat-seal plastic sheets or films. The power dissipated in the polymer is given by [14] (3.69) where Nn= power (W) / = frequency of the alternating field (s"1) C = capacitance of the polymer (farads) E = applied voltage (Volt) 0 = phase angle

The rate of heat generation in a plastic film can be obtained from Equation 3.69 and given as [15] (3.70) where Nn= rate of heat generation (W/m 3 ) £* = dielectric loss factor b = half thickness of the film (\i) Example Given: E / €* b

= 500 V = 10 MHz = 0.24 =50 Ji

Calculate the rate of heat generation and the time required to heat the polymer from 20 0 C to 150 0 C. Substituting the given values in Equation 3.70 gives

The maximum heating rate AT per second is calculated from (3.71) For

Finally the heating time is

3.8

Fick's Law o f Diffusion

Analogous to Fourier's law of heat conduction (Equation 3.1) and the equation for shear stress in shear flow, the diffusion rate in mass transfer is given by Fick's law. This can be written as [16] (3.72) where mA A D^B cA x

= mass flux per unit time - Area = diffusion coefficient of the constituent A in constituent B = mass concentration of component A per unit volume = distance.

The governing expression for the transient rate of diffusion is [2] (3.73) where t = time x = distance The desorption of volatile or gaseous components from a molten polymer in an extruder can be calculated from [17] using Equation 3.73 (3.74) where ^1 Ac C0 D t

= rate of desorption (g/s) = area of desorption (cm2) = initial concentration of the volatile component (g/cm3) in the polymer = diffusion coefficient (cm2/s) - time of exposure (s) of the polymer to the surrounding atmosphere

3.8.1

Permeability

Plastics are permeable by gases, vapors and liquids to a certain extent. The dififiisional characteristics of polymers can be described in terms of a quantity known as permeability.

The mass of the fluid permeating through the polymer at equilibrium conditions is given by [7] (3.75) where m p t A Pv Pi s

- mass of the fluid permeating (g) = permeability [g/(m • s • Pa)] = time of diffusion (s) = area of the film or membrane (m2) = Partial pressures on the side 1 and 2 of the film (Pa) = thickness of the film (mm)

In addition to its dependence on temperature, the permeability is influenced by the difference in partial pressures of the fluid and thickness of the film. Other factors influencing permeability are the structure of the polymer film, such as crystallinity, and the type of fluid. 3.8.2

Absorption and Desorption

The process by which the fluid is absorbed or desorbed by a plastic material is timedependent, governed by its solubility and by the diffusion coefficient [7]. The period until equilibrium value is reached can be very long. Its magnitude can be estimated by the half-life of the process given by [7] (3.76) where t05 = half life of the process s = thickness of the polymer assumed to be penetrated by one side D = diffusion coefficient The value of tQ 5 for moisture in polymethyl methacrylate (PMMA) for and s = 3 mm is 17.1 days when the sheet is wetted from one side only [7]. However, the equilibrium absorption takes much longer, as the absorption rate decreases with saturation.

References [I]

BENDER, E.: Lecture notes, Warme and Stoffiibergang, Univ. Kaiserslautern (1982)

[2]

MCCABE, W. L., SMITH, J. C , HARRIOTT, P.: Unit Operations of Chemical Engineering. McGraw Hill, New York (1985)

[3]

MARTIN, H.: in VDI Warmeatlas, VDI Verlag, Diisseldorf (1984)

[4]

WELTY, J. R., WICKS, C. E., WILSON, R. E.: Fundamentals of Momentum, Heat and Mass Transfer, John Wiley, New York (1983)

[5]

KREITH, E, BLACK, W. Z.: Basic Heat Transfer, Harper & Row, New York (1980)

[6]

THORNE, J. L.: Plastics Process Engineering, Marcel Dekker, New York (1979)

[7]

OGORKIEWICZ, R. M.: Thermoplastics - Properties and Design, John Wiley, New York (1974)

[8]

WUBKEN, G.: Berechnen von Spritzgiefiwerkzeugen, VDI Verlag, Diisseldorf (1974)

[9]

GERSTEN, K.: Einfuhrung in die Stromungsmechanik, Vieweg, Braunschweig (1981)

[ 10] WINTER, H. H.: Extruder als Plastifiziereinheit, VDI Verlag, Diisseldorf (1977) [II] RAUWENDAAL, C.: Polymer Extrusion, Hanser Publishers, Munich (2001) [12] KREMER, H.: Grundlagen der Feuerungstechnik, Engler-Bunte-Institut, Univ. Karlsruhe (1964) [13] COGSWELL, F. N.: Polymer Melt Rheology, George Godwin, London (1981) [ 14] BERNHARDT, E. C.: Processing of Thermoplastic Materials, Reinhold, New York (1959) [15] MCKELVEY, J. M.: Polymer Processing, John Wiley, New York (1962) [16] HOLMAN, J. P.: Heat Transfer, McGraw Hill, New York (1980) [17] SECOR, R. M.: Polym. Eng. ScL 26 (1986) p. 647

4

D e s i g n i n g Plastics

Parts

The deformational behavior of polymeric materials depends mainly on the type and magnitude of loading, time of application of the load, and temperature. The deformation is related to these factors in a complex manner, so that the mathematical treatment of deformation requires a great computational effort [I]. However, in recent times computational procedures for designing plastic parts have been developed using stress-strain data, which were carefully measured by employing computer-aided testing of polymers [2].

4.1

Strength of Polymers

The basic equation for calculating the design stress of a part under load is given by [ 1 ] (4.1) where K av °zui S A

= material strength as a mechanical property = maximum stress occurring in the part ~ allowable stress = factor of safety = material reduction factor

The relation between allowable stress and the polymer-dependent reduction factors can be written as [1] (4.2) The factor A 0 considers the influence of temperature on the strength of the material and can be calculated from [1] (4.3) where 0 = temperature. The limits of applicability of Equation 4.3 are 20 < 0 < 100 0 C. The value k based on the reference temperature of 20 0 C is given for the following materials as[l] PA66 PA6 PBT

=0.0112 = 0.0125 = 0.0095

GR-PA a n d GR-PBT = 0 . 0 0 7 1 POM = 0.0082 ABS =0.0117 The other reduction factors in Equation 4.2 consider the following effects: The factor A st represents the effect of the time of static loading and can have following values depending o n time [ I ] : time

hours

weeks

months

years

Ast

1.3

1.6

1.7

2

The factor A d y n takes the effect of dynamic loading into account and lies in the range of 1.3 to 1.6. The factor A A , considers the influence of aging a n d has to be determined experimentally. The reduction of strength caused by the absorption of moisture by the plastic can be estimated from the factor A w . For unreinforced polyamides A w is roughly [ 1 ] (4.4)

with /ranging from 0 < / < 3 where/= weight percentage of moisture. The value of Aw is 3.4 when/is greater than 3.

4.2

Part Failure

Usually stresses resulting from loading of the part are multiaxial. Because measured material properties do not exist for combined stresses, the multiaxial state has to be reduced to an uniaxial state by applying the principle of equivalence. According to HUBER, VON MISES and HENKY [1] the governing equation for the equivalent stress is (4.5) where CT1, G1 and (T3 are normal stresses. The equivalent strain £ is defined by [3] (4.6) Materials, whose compressive stress is higher than the tensile stress, can be better described by the conical or parabolic criterion [I]. The equivalent stress CT , according to the conical criterion, is given as [ 1 ]

(4.7) The parabolic failure criterion is defined by (4.8)

where m is the ratio of compressive stress to tensile stress. Example Figure 4.1 [1] shows a press fit assembly consisting of a metal shaft and a hub made of POM. The joint strength can be determined as follows: For the numerical values rJrY = 1.6 and p = 22 N/mm 2 the equivalent stress is to be calculated. The tangential stress Gx is given by

Substituing the values above (4.9) The radial compressive stress G1 is

(N]

Figure 4.1 Stress analysis in a press fit hub

Substituting Gx = 50.2 N/mm 2 , G2 = -22 N/mm 2 and G3 = 0 in Equation 4.5 gives

The equivalent stress Cv obtained from

y according

to Equation 4.7 for the conical failure criterion, is

w i t h m = 1.4 for POM. The yield point of POM is around 58 N/mm 2 . Thus, the assumed joint strength is too high. In the case of deformation of the part by shear, the shear stress is given by [I] T = 0.5 O

(4.10)

4.3

T i m e - D e p e n d e n t D e f o r m a t i o n a l Behavior

4.3.1

Short-Term Stress-Strain Behavior

As mentioned in Section 1.4, polymers are viscoelastic materials and their deformational behavior is nonlinear. A typical stress-strain curve of POM under short-term loading is shown in Figure 4.2. Curves of this type can be expressed by a fifth degree polynomial of the form [4] (4.11) where PK0 ... PK5 are polynomial coefficients dependent on the resin at a given temperature.

Stress 6

N/mm2

% Strain £ Figure 4.2

Stress-strain diagram for POM

Stress 6 Figure 4.3

Secant modulus [4]

Strain £

The secant modulus (Figure 4.3) is given by (4.12) Setting PK0 = 0 it follows from Equation 4.11 (4.13) 4.3.2

Long-Term Stress-Strain Behavior

The dimensioning of load bearing plastic components requires knowledge of stress-strain data obtained under long-term loading at different temperatures. Retardation experiments provide data on time-dependent strain in the form of creep plots, see Figure 4.4a. In Figure 4.4b the stress is given as a function of time for different values of strain. Isochronous stress-strain-time curves are illustrated in Figure 4.4c. The critical strain method according to MENGES [10] provides a useful criterion for designing plastic parts. The experiments of MENGES and TAPROGGE [10] show that safe design is possible when the critical strain is taken as the allowable deformation. The corresponding tensile stress can be obtained from the isochronous stress-strain diagram. The expression for calculating the time-dependent strain according to FINDLEY [8] is given as (4.14) The power function of

FINDLEY

[2] is written as (4.15)

The function for the coefficient m is a fifth degree polynomial and that of n is a straight line. With the Findley power function the long-term behavior of plastics up to 105 hours can be described on the basis of measurements covering shorter periods of approx. 103 hours [2].

Strain S

a

Time /

Figure 4.4

Time t Long-term stress-strain behavior [7]

c

Stress 6

Stress 6

b

Strain £

Example [9]

The minimum depth of the simple beam made of SAN shown in Figure 4.5 is to be determined for the following conditions: The beam should support a mid-span load of 11.13 N for 5 years without fracture and without causing a deflection exceeding 2.54 mm.

Figure 4.5

Beam under midspan load [9]

Solution

The maximum stress is given by (4.16)

where P Lybyd

= load (N) = dimensions in (mm) as shown in Figure 4.5

The creep modulus Ec is calculated from (4.17) where /is deflection in mm. The maximum stress from Figure 4.6 after a period of 5 years (= 43800 h) is CJmax 23.44 N/mm 2

Initial applied stress

JL mm2

h Time at rupture Figure 4.6

Creep curve for SAN [9]

Creep modulus

mm2

h Tm iet Figure 4.7

Creep modulus for SAN [9]

Working stress 37 For smaller values of this ratio, Ga1111111118 has to be multiplied by the factor P p given in Figure 5.1. The height H and width W are obtained in this case from Equation 5.6 and Equation 5.7. 5.1.1.2

Shear Rate in Die Channels

The shear rate for the channels treated above can be computed from [3] (5.9)

(5.10)

(5.11) The shear rate for an equilateral triangle is given by [4] (5.12) where d is the half length of a side of the triangle. The relation for a quadratic cross-section is [4] (5.13) where a is the length of a side of the square. In the case of channels with varying cross-sections along the die length, for example, convergent or divergent channels, the channel is divided into a number of sufficiently small increments and the average dimensions of each increment are used in the equations given above [3]. 5.1.1.3

General Relation for Pressure Drop in Any Given Channel Geometry

By means of the substitute radius defined by SCHENKEL [5] the pressure drop in crosssections other than the ones treated in the preceding sections can be calculated. The substitute radius is expressed by [5]

(5.14)

where Rrh= substitute radius A - cross-sectional area B = circumference 5.1.1.4

Examples

The geometrical forms of the dies used in the following examples are illustrated in Figure 5.2. Example 1 It is required to calculate the pressure drop Ap of a LDPE melt at 200 0 C flowing through a round channel, 100 mm long and 25 mm diameter, at a mass flow rate of m = 10 g/s . The constants of viscosity in the Equation 1.36 for the given LDPE are A0 A1 A2 A3 A4

Figure 5.2

= 4.2968 = -3.4709 • 10"1 =-1.1008- 10"1 = 1.4812 • 10"2 =-1.1150-HT 3

Flow channel shapes in extrusion dies

melt density p m = 0.7 g/cm3 Solution Volume flow rate Q = — = — = 14.29 cm 3 /s = 1.429 • 10~5 m 3 /s An 0.7 Shear rate f^ from Equation 5.9:

Shift factor aT from Equation 1.34:

By Equation 1.37, the power law exponent n is

Substituting the constants A1 ... A4 results in n = 1.832 Viscosity 7]a from Equation 1.36

With aT = 0.374, yz = 9.316 and the constants A0 ... A4 we get

Shear stress T from Equation 1.22

Factor of proportionality K from Equation 1.26:

Die constant Gcirde from Equation 5.3:

Pressure drop from Equation 5.2:

Example 2 Melt flow through a slit of width W = 75 mm, height H = 1 mm, and length L = 100 mm. The resin is LDPE with the same viscosity constants as in Example 1. The mass flow rate and the melt temperature have the same values, m = 10 g/s and T = 200 0C. The pressure drop Ap is to be calculated. Solution Volume flow rate Shear rate from Equation 5.10:

Shift factor aT from Equation 1.34: power law exponent n from Equation 1.37: Viscosity 7]a from Equation 1.36: Shear stress T from Equation 1.22: Proportionality factor K from Equation 1.26: Correction factor Fp

As the ratio W/H is greater than 20, the die constant which can be calculated from Equation 5.4 need not be corrected.

and finally the pressure drop Ap from Equation 5.2

Example 3 Melt flow through a slit with width W = 25 mm, height H= 5 mm, and length L = 100 mm. The resin is LDPE with the same viscosity constants as in Example 1. The mass flow rate m = 10 g/s and the melt temperature T = 200 0 C. The pressure drop Ap is to be calculated. Solution Volume flow rate Shear rate ya from Equation 5.10:

Shift factor ar from Equation 1.34:

Power law exponent n from Equation 1.37:

Viscosity 7]a from Equation 1.36:

Shear stress T from Equation 1.22:

Proportionality factor K from Equation 1.26:

Correction factor Fp: As the ratio W/H = 5, which is less than 20, the die constant Gslit has to be corrected. F p from Equation 5.5:

Pressure drop Ap from Equation 5.2:

Example 4 Melt flow through an annulus with an outside radius R0 = 40 mm, an inside radius R1 = 39 mm, and of length L = 100 mm. The resin is LDPE with the same viscosity constants as in Example 1. The process parameters, mass flow rate, and melt temperature remain the same. Solution Volume flow rate Shear rate y^ from Equation 5.11:

Shift factor aT from Equation 1.34:

Power law exponent n from Equation 1.37: n = 2.907 Viscosity 7]a from Equation 1.36: ?7a = 579.43 Pa • s Shear stress T from Equation 1.22: T= 200173.6 N/m 2 Factor of proportionality K from Equation 1.26: K= 1.3410 -10" 13 Correction factor Fp As the ratio G

annuius

from

— = 248.19 is greater than 37, no correction is necessary. Equation 5.8:

Pressure drop Ap from Equation 5.2

Example 5 Melt flow through a quadratic cross section with the length of a side a = 2.62 mm. The channel length L = 50 mm. The resin is LDPE with the following constants for the power law relation in Equation 1.32:

Following conditions are given: mass flow rate melt temperature melt density The pressure drop Ap is to be calculated. Solution Three methods of calculation will be presented to find the pressure drop in this example. Method a With this method, the melt viscosity is calculated according to the power law. Other than that, the method of calculation is the same as in the foregoing examples. Volume flow rate Shear rate For a square with W=H the shear rate yz is

Power law exponent n:

Viscosity rja from Equation 1.32:

Shear stress T from Equation 1.22: T= 40434.88 N/m 2 Proportionality factor K from Equation 1.26: K= 4.568 -1(T14 Correction factor F p W As — = 1 is less than 20, the correction factor is obtained from Equation 5.5 H fp = 1.008 - 0.7474 • 1 + 0.1638 • I 2 = 0.4244 Die constant Gslit from Equation 5.4: Gslit =4.22 • 10"5 G8Ut corrected = 0-4244 • 4.22-10"5 = 1.791 • 10-5 Pressure drop Ap from Equation 5.2:

Method b The shear rate ya is calculated from Equation 5.13

Viscosity ?]a from Equation 1.32: 77a = 24205.54 • 5.67403286"1 = 7546.64 Pa • s Shear stress T from Equation 1.22: T= 42819.6 N/m 2 Power law exponent n from Equation 1.28:

Proportionality factor K from Equation 1.26: K= 4.568 -10" 14 The pressure drop Ap is found from

(5.15)

with the die constant Gsquare

(5.16)

In Equation 5.15

Finally Apsquare from Equation 5.2:

The above relationship for shear rate developed by same result as obtained by Method a.

RAMSTEINER

[4] leads to almost the

Method c In this method, a substitute radius is calculated from Equation 5.14; the pressure drop is then calculated using the same procedure as in the case of a round channel (Example 1): Substitute radius .Rrh:

Shear rate % from Equation 5.13:

Viscosity ?]a from Equation 1.32: 7]a = 24205.54 • 7.1830'3216"1 = 6441.56 Pa • s Shear stress T from Equation 1.22: T = 46269.73 N/m 2 Factor of proportionality from Equation 1.26: K = 4.568- 10"14 ^circle fr°m Equation 5.3:

Pressure drop from Equation 5.2:

This result shows that the relationship, Equation 5.14 [5], is sufficiently accurate for practical purposes. This equation is particularly useful for dimensioning channels, whose geometry differs from the common shape, that is, circle, slit or annulus. The procedure of calculation for an equilateral triangle is shown in the following example: Example 6 Melt flow through an equilateral triangular channel of length L = 50 mm. The side of the triangle 2 d = 4.06 mm. Other conditions remain the same as in Example 5. Solution Substitute radius Rrh from Equation 5.14 with

n = 3.043 RTh= 1.274 mm Shear rate / a from Equation 5.9:

Viscosity 7]a from Equation 1.32: 77a = 24205.54 • 8.8 0 ' 3 2 8 " = 5620.68 Pa • s Shear stress T from Equation 1.22: T= 49462 N/m 2 Factor of proportionality from Equation 1.26: K= 4.568-10"14 Gcircle from Equation 5.3:

Pressure drop Ap from Equation 5.2:

Using the relation developed by RAMSTEINER [4] on the basis of rheological measurement on triangular channels, Example 6 is calculated as follows for the purpose of comparing both methods: Shear rate from Equation 5.12:

Viscosity 7]a from Equation 1.32: 7]a = 24205.54 • 5.6920'3286"1 = 7530.61 Pa • s Shear stress T from Equation 1.22: T = 42864.2 N/m 2 Factor of proportionality from Equation 1.26: K= 4.568 -10" 14

Die constant Gtriangle: (5.17)

Pressure drop Ap from Equation 5.2:

This result differs little from the one obtained by using the concept of substitute radius. Therefore this concept of SCHENKEL [5] is suitable for use in practice. 5.1.1.5

Temperature Rise and Residence Time

The adiabatic temperature increase of the melt can be calculated from (5.18) where AT Ap pm cpm

= = = =

temperature rise (K) pressure difference (bar) melt density (g/cm 3 ) specific heat of the melt kj/(kg • K)

The residence time T of the melt in the die of length L can be expressed as (5.19) u = average velocity of the melt Equation 5.19 for a tube can be written as

(5.20) R = tube radius ya = shear rate according to Equation 5.9

The relation of a slit is (5.21) H = height of slit ya = shear rate according to Equation 5.10 5.1.1.6

Adapting Die Design to Avoid Melt Fracture

Melt fracture can be defined as an instability of the melt flow leading to surface or volume distortions of the extrudate. Surface distortions [34] are usually created from instabilities near the die exit, while volume distortions [34] originate from the vortex formation at the die entrance. Melt fracture caused by these phenomena limits the production of articles manufactured by extrusion processes. The use of processing additives to increase the output has been dealt with in a number of publications given in [35]. However, processing aids are not desirable in applications such as pelletizing and blow molding. Therefore, the effect of die geometry on the onset of melt fracture was examined. The onset of melt fracture with increasing die pressure is shown for LDPE and HDPE in Figure 5.3 [38]. As can be seen, the distortions appear differently depending on the resin. The volume flow rate is plotted in Figure 5.4 [39] first as a function of wall shear stress and then as a function of pressure drop in the capillary for LDPE and HDPE. The sudden increase in slope is evident for LDPE only when the flow rate is plotted against pressure, whereas in the case of HDPE it is the opposite. In addition, for HDPE the occurrence of melt fracture depends on the ratio of length L to diameter D of the capillary. The effect of temperature on the onset of melt fracture is shown in Figure 5.5 [36]. With increasing temperature the onset of instability shifts to higher shear rates. This behavior is used in practice to increase the output. However, exceeding the optimum processing temperature can lead to a decrease in the quality of the product in many processing operations. From these considerations it can be seen that designing a die by taking the resin behavior into account is the easiest method to obtain quality products at high throughputs. Design procedure Using the formulas given in this book and in reference [33], the following design procedure has been developed to suit the die dimensions to the melt flow properties of the resin to be processed with the die. STEP 1: Calculation of the shear rate in the die channel STEP 2: Expressing the measured viscosity plots by a rheological model STEP 3: Calculation of the power law exponent STEP 4: Calculation of the shear viscosity at the shear rate in Step 1 STEP 5: Calculation of the wall shear stress STEP 6: Calculation of the factor of proportionality STEP 7: Calculation of die constant

N/mm2

LDPE

HDPE

Figure 5.3

lrregularties of the extrudate observed at increasing extrusion pressure with LDPE and HDPE [38] InQ

InQ

In

Thank you for interesting in our services. We are a non-profit group that run this website to share documents. We need your help to maintenance this website.

To keep our site running, we need your help to cover our server cost (about $400/m), a small donation will help us a lot.